Abstract
The article investigates the effect of thermal modification of porous carbon material (PCM), obtained from plant feedstock, on its morphology and fractal structure by smallangle Xray scattering (SAXS) method. The analysis of the scattering intensity curves serve the basis for calculating the parameters of the PCM porous structure: the Porod constant, the Porod invariant, average pore radius, specific surface area, and mass and surface fractal dimensions. It has been found out that the PCMs obtained have fractal structure, formed from mass and surface fractals, the sizes of which increase at the growth of temperature and modification time.
PACS
81.05.Uw; 61.05.cf; 82.47.Aa
Keywords:
Porous carbon material; Smallangle Xray scattering; Mass and surface fractalsBackground
One of the principal ways to improve the existing and create new electrochemical technologies is the development of new electrode materials, possessing necessary properties: high electrocatalytic activity, stability, and abundance of original components [1]. These requirements can be provided by creating electrodes on the porous carbon material (PCM) bases that are actively used as electrode materials for primary and secondary chemical power sources and supercapacitors [27]. In particular, we have found out that the specific capacity of lithium power sources on the PCM bases, obtained by hydrothermal carbonization of apricot pits at different temperatures, depends mainly on its specific area and electrical conductivity [8,9]. The maximum value of specific capacity (1.138 mА · h/g) has the electrochemical system on the basis of PCM, obtained at the carbonization temperature of 750°С. It is evident that to increase the specific energy characteristic of the elements, it is necessary to perform intentional change of PCM structure and morphology by means of different types of processing and modification. The most common ways of modification are thermal, chemical, and laser modifications of PCMs [1012]. To study changes caused by such modifications a wide range of methods are currently used: Xray diffraction method [13], smallangle Xray scattering (SAXS) [1416], smallangle neutron scattering [1618], gas adsorption/desorption [1921], scanning tunnel microscopy [22], atomic force microscopy [23], and transmission electron microscopy [24]. Each of these methods has its advantages and disadvantages, but they provide a possibility to obtain important information about the porous structure of the materials (specific area, total pore volume, micropore volume, dimensions and forms of pores, their size distribution, fractal structure, etc.). The advantages of SAXS method, in comparison with other methods, may include the following [25,26]: (1) it is sensitive to both closed and open porosity, (2) SAXS intensity profiles are sensitive to shape and orientation of the scattering, (3) the method can be used to investigate samples that are saturated with liquids, (4) it can be used to investigate the pore texture of materials under operating conditions. Thus, the aim of the work is to perform thermal modification of PCM at different temperatures and times and to investigate the effect of this modification on its morphology and fractal structure using the SAXS method.
Methods
The initial standard was PCM, obtained by method of hydrothermal carbonization of plant material at a temperature of 750°С. It was modified at temperatures Т_{mod} 300°C, 400°C, 500°C (modification time t_{mod} was 0.5, 1, 1.5, 2, 2.5, and 3 h), and 600°С (t_{mod} was 0.25, 0.5, 0.75, and 1 h) in the air in a muffle furnace SNOL40/1300. Less PCM modification times at the temperature 600°С can be explained by the fact that at the given temperature, further thermal treatment leads to the complete material burnoff.
To determine the structural parameters of the materials investigated, the SAXS method
was applied, as it is widely used to study structural heterogeneities of nanometric
scope in disperse systems, including porous materials [27]. SAXS experiments were performed using Xray diffractometer in CuK_{α} radiation (λ = 1.5418 Ǻ), monochromated by reflection from the (200) plane of LiF monocrystal,
as Xray beam passed through the standard. To restrict the parasitic scattering from
the monocrystal monochromator and entrance slits and to reduce the intensity of the
background scattering, the collimators of primary and scattered beams were used. The
collimation system allows to measure SAXS spectra, starting with s = 0.015 Ǻ^{−1} (where
where I^{*}(2θ) is the actual scattering intensity, I_{exp}(2θ) is the experimental scattering intensity, I_{0}(2θ) is the intensity distribution in the primary beam, and T = I_{exp}(0) / I_{0}(0) is the transmission coefficient (intensity proportion of the primary beam, passing through the standard at the zero position of detector). The obtained scattering intensity curves include the collimation adjustment for altitude of the detector receiving slit.
Results and discussion
As follows from the SAXS results, the obtained spectra are in the form of curves, monotonously decaying in the whole angular measurement interval. It indicates the chaotic distribution of the scattering heterogeneities (pores) and respectively the absence of correlation in their relative positions (Figure 1).
Figure 1. SAXS spectra of PCMs (modification time is 1 h).
To determine the parameters, characterizing the porous structure of the materials investigated, the original scattering intensity curves were analyzed. The following asymptotic Porod approximation is correct for the slit collimation system:
describing the behavior of the scattering intensity curves for large s. The parameter σ characterizes the state of the interphase surface. In particular, for σ = 0, the pore surface is smooth, for σ < 0 the surface is diffuse, and the value σ > 0 indicates the existence of fluctuations in the electron density of the material, which is characteristic of fractal objects. If there is the dependence ln {s^{4}I(s)} vs. s^{2}, it will described by linear function at large s (Figure 2). The extrapolation of this linear dependence to s = 0 allows us to find the Porod constant K_{p}.
Figure 2. To definition of Porod constant.
If the Porod constant K_{p} is known, the Porod integral invariant Q may be calculated by the formula
To calculate the effective micropore radius R_{p} and the specific surface area S_{п}, the following formulae were used:
where ρ_{m} is the actual material density that in turn depends on the structural material density ρ_{x} and porosity w according to the equation ρ _{m} = (1 − w) ρ _{x} (structural material density is about 2 g/cm^{3}).
The results of the calculations conducted for PCM, modified at 300°С, show the nonmonotonous changes in parameters of the porous structure (Table 1). The pore volume and pore surface area reach the greater value after modification for 1.5 h. In this case, the pore radius decreases up to 1.7 nm. The shape of the intensity curves of the initial standard and modified ones is similar. As can be seen from the curves in Figure 3, there are linear sections on the intensity curves the slope of which is in the range of 1 < n < 3. This result indicates the fractal distribution of heterogeneities. The samples contain the generated smallscale volumetric fractal structure, formed by carbon nanoclusters, the size of which can be calculated by the formula L_{1} ≈ 2 π / s_{2}, where s_{2} is the lower limit of the fractal mode on the scale s.
Table 1. The parameters of porous and fractal structure of PCM modified at 300°C
Figure 3. SAXS curves in double logarithmical coordinates. Initial PCM (a) and modified ones at 300°C for 0.5 h (b), 1 h (c), 1.5 h (d), 2 h (e), 2.5 h (f), and 3 h (g).
In addition to the smallscale structure, there forms the largescale cluster structure, formed by clusters with the size of L > L_{1} ≈ 2 π / s_{1}. The scattering from those clusters is observed in the range s < s_{1}. The slope of the linear section at s < s_{1} is in the range 3 < n < 4, which indicates the formation of the fractal surface of largescale carbon clusters.
As can be seen from Table 1, the fractal dimension of the cluster surface increases at the increase of material modification time. It should be noted that there are no linear section on the intensity curve of the sample modified for 1 h; that is probably the evidence of the chaotic (nonfractal) distribution of heterogeneities.
The increase of the modification temperature to 400°С and 500°С leads to the substantial change of the parameters of the porous structure of carbon materials in comparison to that modified at 300°С. The most substantial changes at the mentioned modification temperatures can be observed at the modification times 1.5 ÷ 3 h (Tables 2 and 3). First of all, it depends upon the increase of the porosity value resulting from the partial burnoff in the nearsurface layers of the carbon particles and decrease of the PCMs' actual density.
Table 2. The parameters of porous and fractal structure of PCM modified at 400°C
Table 3. The parameters of porous and fractal structure of PCM modified at 500°C
Let us analyze the changes in the parameters of the PCM fractal structure modified at temperature 400°С (scattering intensity curves in double logarithmic coordinates for PCMs, modified at temperatures 400°С, 500°С, and 600°С, are not provided in the article, as their forms are similar to the dependences lg I(s) = f{lg(s)} in Figure 3).
The intensity curve of the sample, modified for 0.5 h, represents the linear section, the slope of which n_{1} = 2.4 indicates the formation of the volumetric fractal structure with the dimension of D_{v} = 2.4. A similar situation can be observed for the initial standard. One can assume that in the range of wave vectors (s_{1}, s_{2}), there is the scattering of nanoclusters, the sizes of which can be calculated by the formula L_{0} ≈ 2 π / s_{2} ≈ 7 nm. In the range s < s_{1}, the linear section may be observed, the slope of which n_{2} = 2.8 indicates the formation of another system of fractal clusters with the size of L ≈ 2 π / s_{1} ≈ 20 nm, the distribution of which is of the volumetric character.
Thermal modification for 1 h leads to the substantial change of the fractal structure.
On the intensity curve in a wide range of scattering angles, there is the linear section
with the slope n_{2} = 3.3. Such shape of the scattering intensity is characteristic of the porous twophase
system (carbon matrix pore) with fractal interphase surface. In this case, the dimension
of the fractal surface is D_{s} = 6 − n_{2} = 2.7 (Table 2). Departure from linearity at small scattering angles (s < s_{1}) is caused by the transition to the Guinier mode, for which the dependence I(s) is described by the formula
In the range of s > s_{2}, there is scattering of monodisperse heterogeneities with the size of r_{c}. Similarly, the scattering at s > s_{2} is described by the Guinier formula. One can assume that the objects investigated are formed by the carbon clusters with the radius R_{c} and with the extended surface, which in turn, consist of nanoclusters with the radius r_{c}. Thus, the values r_{c} and R_{c} define the lower and upper limits of the selfsimilarity of fractal surface. Further increase of the PCM modification time results in quantitative changes in structural parameters. In particular, the fractal dimension of the interphase surface increases, and modification for 2.5 to 3 h leads to the transition from fractal boundary to smooth one with the dimension of D_{s} = 2. Besides, there is the increase in the sizes of carbon nanoparticles r_{c} and fractal clusters R_{c} (Table 2).
In case of PCM, modified at 500°С, the scattering intensity curves are characterized by the linear section in the wide range of scattering angles, the slope of which changes within the limits 3 < n_{2} < 4. Such values n_{2} indicate on the scattering by the fractal surface with the dimension D_{s} = 6 – n_{2}. In this case, the materials investigated can be also viewed as twophase porous systems with the fractal interphase surface. The increase of the modification time leads to the decrease of the fractal dimension and transition to smooth interphase surface (D_{s} = 2) after modification for 2 h. It should be noted that the shape of the intensity curves for PCMs, modified at 400°С and 500°С, is similar. Thus, thermal modification at those temperatures leads to the formation of PCMs, formed by carbon clusters with the radius R_{c} and fractal surface, which in turn, consist of nanoclusters with the radius r_{c} (Table 3).
Thermal modification of the initial standard at 600°С, as compared to the treatment at 400°C and 500°С, leads to a more significant increase of the pore specific volume and surface area at the same modification times because of a higher heattreatment temperature (Table 4). The analysis of the scattering intensity curves in double logarithmic coordinates shows the scattering at the interphase fractal surface with the dimension D_{s} = 2.55 ÷ 2.60. It is characteristic that the increase of the modification time does not change the fractal dimension of the surface. Thus, the objects investigated can be viewed also as twophase porous structures, produced by the carbon clusters with the radius R_{c}, formed from nanoclusters with the radius r_{c}, and pores with the extended fractal surface.
Table 4. The parameters of porous and fractal structure of PCM modified at 600°C
Conclusions
The thermal modification of the initial material at temperature 300°С results in the formation of PCM with the fractal structure, formed by mass fractals with the dimension D_{v} = 2.4 ÷ 2.7, which combine in the surface fractal aggregates with the dimension D_{s} = 2.2 ÷ 2.7. The increase of the modification time leads to the growth in the sizes of both types of fractals.
The increase of the modification temperature to 400°С and 500°С leads to the increase of the pore volume and pore surface area. PCM, modified for 0.5 and 1 h, was formed by carbon clusters with the radius R_{c}, which consists of the nanoclusters with the radius r_{c}. The increase of the modification duration not only leads to the growth in the sizes of carbon nanoparticles and fractal clusters but also causes the transition from fractal to smooth boundary surface (D_{s} = 2) at t_{mod} = 2.5 to 3 h.
Thermal treatment at 600°С and less process duration leads to more substantial changes in the pore specific volume and surface area, the maximum of which is observed at t_{mod} = 0.75 h. Besides, PCM are the twophase porous structures, produced by carbon clusters, formed from nanoclusters, and pores with the extended fractal surface. The increase of the modification duration does not change the surface fractal dimension (D_{s} = 2.55 ÷ 2.60).
Abbreviations
PCM: porous carbon material; SAXS: smallangle Xray scattering.
Competing interests
The authors declare that they have no competing interests.
Authors’ contributions
BKO performed the problem definition and participated in the discussion of the experimental results. VIM stated the choice method and subjects of investigation, participated in the analysis and interpretation of data, and wrote the paper. YOK designed and performed the SAXS experiment and calculated the parameters of PCM porous structure. NIN fabricated the initial standard and performed its thermal modification. All authors read and approved the final manuscript.
Authors’ information
BKO is the corresponding member, a professor at the Physics and Technology Department, Vasyl Stefanyk PreCarpathian National University, IvanoFrankivsk, Ukraine. VIM is an associate professor at the Physics and Technology Department, Vasyl Stefanyk PreCarpathian National University, IvanoFrankivsk, Ukraine. YOK is a senior researcher at the Physics Department, Ivan Franko National University, Lviv, Ukraine. NIN is scientific researcher at the Physics and Technology, Vasyl Stefanyk PreCarpathian National University, IvanoFrankivsk, Ukraine.
Acknowledgements
This work was supported by CRDF/USAID (no. UKX29200IF08) and the Ministry of Education of Ukraine (no. М/1302009).
References

Tarasevich МR: Electrochemistry of Carbon Materials. Moskow: Nauka; 1984.

Zaghib K, Tatsurni K, Abe H, Ohsaki T, Sawada Y, Higuchi S: Optimization of the dimensions of vaporgrown carbon fibber for use as negative electrodes in lithiumion rechargeable cells.
J Electrochem Soc 1998, 145:210215. Publisher Full Text

Basu S: Early studies on anodic properties of lithium intercalated graphite.

Ogumi Z, Inaba M: Carbon anodes. In Advances in LithiumIon Batteries. Edited by van Schalkwijk WA, Scrosati B. New York: Kluwer; 2002:79101.

Noel M, Suryanarayanan V: Role of carbon host lattices in Liion intercalation/deintercalation processes.
J Power Sources 2002, 111(2):193209. Publisher Full Text

Novak P, Goers D, Spahr ME: Carbon materials in lithiumion batteries. In Carbons for Electrochemical Energy Storage Systems. Edited by Béguin F, Frackowiak E. Boca Raton: CRC; 2002:263328.

Conway BE: Electrochemical Supercapacitors. Scientific Fundamentals and Technological Applications. New York: Kluwer; 1999.

Nagirna NI, Mandzyuk VI, Lisovskyy RP, Rachiy BI, Merena RI: Electrochemical insertion of lithium ions into porous carbon materials. In undamentals Problems of Energy Transformation in Lithium Electrochemical Systems: Materials of XII International Conference, October 2012; Krasnodar, Russia. Edited by Galkin VV. Krasnodar: Kuban State University; 2012:188190.

Mandzyuk VI, Nagirna NI, Strelchuk VV, Budzulyak SI, Budzulyak ІМ, Myronyuk ІF, Rachiy BI: Electrical and optical properties of porous carbon material.

Dahn JR, Zheng T, Liu Y, Xue JS: Mechanisms for lithium insertion in carbonaceous materials.
Science 1995, 270(5236):590593. Publisher Full Text

Ostafiychuk BК, Budzulyak ІМ, Rachiy BI, Merena RI, Magometa OD: The effect of chemical treatment on properties of activated carbon materials.

Berkeshchuk МV, Budzulyak ІМ, Lisovskyy RP, Merena RI: Thermochemical and laser modification of nanoporous carbon for electrochemical capacitor electrodes.

Fey GTK, Cho YD, Chen CL, Huang KP, Lin YC, Kumar TP, Chan SH: Pyrolytic carbons from porogentreated rice husk as lithiuminsertion anode materials.

Pikus S, Kobylas E: Small angle Xray study of coated porous materials.
Coll Surf A Physicochem Eng Aspects 2002, 208:219229. Publisher Full Text

Oliveira MHJ, Barbieri PF, Torriani IL, Marques FC: SAXS analysis of graphitic amorphous carbon.
Thin Solid Films 2007, 516:316319. Publisher Full Text

Radlinski AP, Mastalerz M, Hinde AL, Hainbuchner M, Rauch H, Baron M, Lin JS, Fan L, Thiyagarajan P: Application of SAXS and SANS in evaluation of porosity, pore size distribution and surface area of coal.
Int J Coal Geol 2004, 59:245271. Publisher Full Text

Avdeev МА, Balogoveshchensky НМ, Martynov PN, Melnikov VP, Novikov AG, Puchkov AV: The investigation of activated carbon microstructure by smallangle slow neutron scattering method.

Bogdanov SG, Valiev EZ, Pirogov АN: The fractal structure of carbon fibbers.

Gregg SJ, Sing KSW: Аdsorption, Surface Area and Porosity. London: Academic; 1982.

Karnaukhov АP: Аdsorption. Texture of Dispersed and Porous Materials. Novosibirsk: Nauka; 1999.

Rouquerol F, Rouquerol J, Sing KSW: Adsorption by Powders & Porous Solids. London: Academic; 1999.

Almquist N: Fractal analysis of scanning probe microscopy images.

Kim CH, Pyun SI, Kim JH: An investigation of the capacitance dispersion on the fractal carbon electrode with edge and basal orientations.
Electrochim Acta 2003, 48(23):34553463. Publisher Full Text

Pyun SI, Rhee CK: An investigation of fractal characteristics of mesoporous carbon electrodes with various pore structures.
Electrochim Acta 2004, 49:41714180. Publisher Full Text

Hoinkis S: Smallangle scattering of neutrons and Xrays from carbons and graphites. In Chemistry and Physics of Carbon 25. Edited by Thrower PA. New York: Marcel Dekker; 1997:71241.

Calo JM, Hall PJ, Houtmann S, LozanoCastelló D, Winans RE, Seifert S: “Real time” determination of porosity development in carbons: a combined SAXS/TGA approach. In Studies in Surface Science and Catalysis, Characterisation of Porous Solids IV. Volume 144. Edited by RodriguezReinoso F, McEnaney B, Rouquerol J, Unger K. Amsterdam: Elsevier Science; 2002:5966.

Svergun DI, Feygin LА: Xray and Neutron SmallAngle Scattering. Moskow: Nauka; 1986.